Smart composite films of nanometric thickness based on copper-iodine coordination polymers. Toward sensors.
Conesa-Egea, Javier; Nogal, Noemí; Martínez, José Ignacio; Fernández-Moreira, Vanesa; Rodríguez-Mendoza, Ulises R; González-Platas, Javier; Gómez-García, Carlos J; Delgado, Salomé; Zamora, Félix; Amo-Ochoa, Pilar; Chemical science 9 (2018) 8000–8010; doi:10.1039/c8sc03085e

data_1549830
_publ_section_title
;
 Smart composite films of nanometric thickness based on copper-iodine
 coordination polymers. Toward sensors.
;
_journal_issue                   41
_journal_name_full               'Chemical science'
_journal_page_first              8000
_journal_page_last               8010
_journal_paper_doi               10.1039/c8sc03085e
_journal_volume                  9
_journal_year                    2018
_chemical_formula_moiety         'C7 H8 Cu I N2 O2'
_chemical_formula_sum            'C7 H8 Cu I N2 O2'
_chemical_formula_weight         342.59
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     dual
_audit_creation_date             2017-07-10
_audit_creation_method
;
Olex2 1.2
(compiled 2017.03.28 svn.r3405 for OlexSys, GUI svn.r5337)
;
_audit_update_record
;
2018-03-01 deposited with the CCDC.
2018-08-23 downloaded from the CCDC.
;
_cell_angle_alpha                85.828(12)
_cell_angle_beta                 88.899(7)
_cell_angle_gamma                85.395(13)
_cell_formula_units_Z            2
_cell_length_a                   4.0680(3)
_cell_length_b                   9.2600(18)
_cell_length_c                   10.9110(10)
_cell_measurement_reflns_used    1024
_cell_measurement_temperature    296(1)
_cell_measurement_theta_max      24.9200
_cell_measurement_theta_min      3.7360
_cell_volume                     408.56(9)
_computing_cell_refinement       'CrysAlisPro 1.171.38.46 (Rigaku OD, 2015)'
_computing_data_collection       'CrysAlisPro 1.171.38.46 (Rigaku OD, 2015)'
_computing_data_reduction        'CrysAlisPro 1.171.38.46 (Rigaku OD, 2015)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'ShelXT (Sheldrick, 2015)'
_diffrn_ambient_pressure         3080000(40000)
_diffrn_ambient_temperature      296(1)
_diffrn_detector                 'CCD plate'
_diffrn_detector_area_resol_mean 16.2536
_diffrn_detector_type            EosS2
_diffrn_measured_fraction_theta_full 0.355
_diffrn_measured_fraction_theta_max 0.355
_diffrn_measurement_details
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  t~exp~   \w     \q     \k     \f   Frames
  1  \w    -29.00   4.00   0.50   30.00    --   26.32  26.00  -7.00   66
  2  \w    -35.00  -5.00   0.50   30.00    --   26.32 114.00 -45.00   60
  3  \w     -4.00  35.00   0.50   30.00    --   26.32 -53.00  17.00   78
  4  \w    -45.00 -17.00   0.50   30.00    --   26.32 134.00 123.00   56
  5  \w    -14.00  45.00   0.50   30.00    --   26.32 -26.00-172.00  118
  6  \w    -96.00 -45.00   0.50   30.00    --  -27.02 134.00 123.00  102
  7  \w    -11.00  15.00   0.50   30.00    --  -27.02 -81.00  29.00   52
  8  \w    -31.00  33.00   0.50   30.00    --  -27.02 -26.00   7.00  128
  9  \w    -55.00 -17.00   0.50   30.00    --  -27.02  67.00 -23.00   76
 10  \w    -27.00  19.00   0.50   30.00    --  -27.02 -39.00-167.00   92
 11  \w    -52.00  17.00   0.50   30.00    --  -27.02  39.00 167.00  138
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'SuperNova, Dualflex, EosS2'
_diffrn_measurement_method       '\w scans'
_diffrn_orient_matrix_type
'CrysAlisPro convention (1999,Acta A55,543-557)'
_diffrn_orient_matrix_UB_11      0.0116611000
_diffrn_orient_matrix_UB_12      -0.0762600000
_diffrn_orient_matrix_UB_13      0.0138414000
_diffrn_orient_matrix_UB_21      0.1666651000
_diffrn_orient_matrix_UB_22      -0.0042124000
_diffrn_orient_matrix_UB_23      -0.0206467000
_diffrn_orient_matrix_UB_31      0.0518796000
_diffrn_orient_matrix_UB_32      0.0101185000
_diffrn_orient_matrix_UB_33      0.0602607000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0521
_diffrn_reflns_av_unetI/netI     0.0473
_diffrn_reflns_Laue_measured_fraction_full 0.355
_diffrn_reflns_Laue_measured_fraction_max 0.355
_diffrn_reflns_limit_h_max       4
_diffrn_reflns_limit_h_min       -4
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_k_min       -4
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            1885
_diffrn_reflns_point_group_measured_fraction_full 0.355
_diffrn_reflns_point_group_measured_fraction_max 0.355
_diffrn_reflns_theta_full        24.963
_diffrn_reflns_theta_max         24.963
_diffrn_reflns_theta_min         1.872
_diffrn_source                   'fine-focus sealed X-ray tube'
_diffrn_source_type              'Enhance (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    6.413
_exptl_absorpt_correction_T_max  0.293
_exptl_absorpt_correction_T_min  0.222
_exptl_absorpt_correction_type   gaussian
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.38.46 (Rigaku Oxford Diffraction, 2015)
Numerical absorption correction based on gaussian integration over
            a multifaceted crystal model (Absorb Angel (2004) J. Appl. Cryst. 37:486-492)
;
_exptl_crystal_colour            orange
_exptl_crystal_colour_primary    orange
_exptl_crystal_density_diffrn    2.785
_exptl_crystal_description       plate
_exptl_crystal_F_000             324
_exptl_crystal_preparation       'mounted in a diamond-anvil cell '
_exptl_crystal_size_max          0.091
_exptl_crystal_size_mid          0.04
_exptl_crystal_size_min          0.02
_refine_diff_density_max         0.702
_refine_diff_density_min         -0.771
_refine_diff_density_rms         0.172
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.116
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     52
_refine_ls_number_reflns         506
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.116
_refine_ls_R_factor_all          0.0541
_refine_ls_R_factor_gt           0.0425
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0764P)^2^+0.1388P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1106
_refine_ls_wR_factor_ref         0.1194
_reflns_Friedel_coverage         0.000
_reflns_number_gt                431
_reflns_number_total             506
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c8sc03085e2.cif
_cod_data_source_block           JCE140CS_308GPa
_cod_depositor_comments
'Adding full bibliography for 1549820--1549832.cif.'
_cod_database_code               1549830
_shelx_shelxl_version_number     2017/1
_exptl_oxdiff_absorpt_process_details
;
Gaussian integration over a grid
of 16 x 16 x 16 points =  4096 total grid points
  Based upon method of Burnham (1966)

 Data corrected for diamond-anvil cell absorption
 Note that exptl_absorpt_correction_tmin and _tmax
 the total correction factors applied to the intensities
 The individual factors are:
         range of dac transmission factors (min-max)      0.274     0.352
         range of gasket transmission (min-max)           0.997     1.000
         range of P media transmission (min-max)          1.000     1.000

 thickness of diamond anvil 1: 15.500 mm, mu =  0.0202 mm-1
       thickness of platten 1: 44.000 mm, mu =  0.0047 mm-1

 thickness of diamond anvil 2: 15.500 mm, mu =  0.0202 mm-1
       thickness of platten 2: 44.000 mm, mu =  0.0047 mm-1

    Gasket shadowing corrections were made based upon
    Gasket thickness =  50.0 microns, radius = 107.0 microns
    Gasket absorption coeff =        21.00 mm-1
    REFLECTION WAS CONSIDERED TOTALLY OBSCURED IF
 FRACTION CRYSTAL ILLUMINATED WAS LESS THAN 0.00

    Non-absorbing pressure medium
;
_reflns_odcompleteness_completeness 35.31
_reflns_odcompleteness_iscentric 1
_reflns_odcompleteness_theta     24.97
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups, All N(H,H) groups
 At 1.5 times of:
  All C(H,H,H) groups
2.a Aromatic/amide H refined with riding coordinates:
 C5(H5), C4(H4), C2(H2)
2.b Fitted hexagon refined as free rotating group:
 N1(C5,C4,C3,C2,C1)
2.c X=CH2 refined with riding coordinates:
 N2(H2A,H2B)
2.d Idealised Me refined as rotating group:
 C7(H7A,H7B,H7C)
;
_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
;
_oxdiff_exptl_absorpt_empirical_full_max 2.805
_oxdiff_exptl_absorpt_empirical_full_min 0.601